Solid-State Nonlinear Optical Switch with the Widest Switching Temperature Range Owing to Its Continuously Tunable <i>T</i><sub>c</sub>.
Pan, Chun-Ya; Yang, Xin-Rui; Xiong, Lin; Lu, Zhong-Wei; Zhen, Bo-Yu; Sui, Xin; Deng, Xue-Bin; Chen, Ling; Wu, Li-Ming; Journal of the American Chemical Society 142 (2020) 6423–6431; doi:10.1021/jacs.0c01741

data_4134477
_publ_section_title
;
 Solid-State Nonlinear Optical Switch with the Widest Switching
 Temperature Range Owing to Its Continuously Tunable <i>T</i><sub>c</sub>.
;
_journal_issue                   13
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              6423
_journal_page_last               6431
_journal_paper_doi               10.1021/jacs.0c01741
_journal_volume                  142
_journal_year                    2020
_chemical_formula_sum            'F H6.45 K0.39 N1.61 O3 P'
_chemical_formula_weight         142.22
_space_group_IT_number           33
_space_group_name_Hall           'P 2c -2n'
_space_group_name_H-M_alt        'P n a 21'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   7.9345(9)
_cell_length_b                   11.0298(13)
_cell_length_c                   5.9653(8)
_cell_measurement_temperature    273(2)
_cell_volume                     522.06(11)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      273(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.994
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0616
_diffrn_reflns_av_sigmaI/netI    0.0352
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            9949
_diffrn_reflns_theta_full        27.52
_diffrn_reflns_theta_max         27.52
_diffrn_reflns_theta_min         3.16
_exptl_absorpt_coefficient_mu    0.767
_exptl_crystal_density_diffrn    1.809
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             292
_refine_diff_density_max         0.365
_refine_diff_density_min         -0.371
_refine_diff_density_rms         0.082
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.13(19)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.139
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     89
_refine_ls_number_reflns         1189
_refine_ls_number_restraints     39
_refine_ls_restrained_S_all      1.123
_refine_ls_R_factor_all          0.0518
_refine_ls_R_factor_gt           0.0463
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0357P)^2^+0.8612P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0979
_refine_ls_wR_factor_ref         0.1002
_reflns_number_gt                1099
_reflns_number_total             1189
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            K0.5(NH4)1.5PO3F.cif
_cod_data_source_block           K0.5(NH4)1.5PO3F-300K
_cod_depositor_comments
'Adding full bibliography for 4134470--4134505.cif.'
_cod_original_formula_sum        'H6.45 F K0.39 N1.61 O3 P'
_cod_database_code               4134477